An efficient magnetically modified microbial cell biocomposite for carbazole biodegradation
© Li et al.; licensee Springer. 2013
Received: 2 September 2013
Accepted: 4 December 2013
Published: 11 December 2013
Magnetic modification of microbial cells enables to prepare smart biocomposites in bioremediation. In this study, we constructed an efficient biocomposite by assembling Fe3O4 nanoparticles onto the surface of Sphingomonas sp. XLDN2-5 cells. The average particle size of Fe3O4 nanoparticles was about 20 nm with 45.5 emu g-1 saturation magnetization. The morphology of Sphingomonas sp. XLDN2-5 cells before and after Fe3O4 nanoparticle loading was verified by scanning electron microscopy and transmission electronic microscopy. Compared with free cells, the microbial cell/Fe3O4 biocomposite had the same biodegradation activity but exhibited remarkable reusability. The degradation activity of the microbial cell/Fe3O4 biocomposite increased gradually during recycling processes. Additionally, the microbial cell/Fe3O4 biocomposite could be easily separated and recycled by an external magnetic field due to the super-paramagnetic properties of Fe3O4 nanoparticle coating. These results indicated that magnetically modified microbial cells provide a promising technique for improving biocatalysts used in the biodegradation of hazardous compounds.
KeywordsCarbazole Immobilization Nanoparticles Biodegradation Reusability
As types of toxic and mutagenic common nitrogen compounds, carbazole and its derivatives readily undergo radical chemistry to generate the more poisonous hydroxynitrocarbazoles [1–4]. Soil, river sediments, and ground water polluted by carbazole have become a great threat to the environment. Therefore, it is necessary to establish effective methods to clear up carbazole and its derivatives.
Nanoscale iron particles represent a new generation of environmental remediation technologies that could provide cost-effective solutions to some of the most challenging environmental cleanup problems . Due to biocompatibility, large surface areas, high surface reactivity, and super-paramagnetic properties, nanoscale iron particles provide enormous flexibility for environmental applications [6–8]. Research has shown that nanoscale iron particles are very effective for the transformation and detoxification of a wide variety of common environmental contaminants, such as hazardous organic compound [9–11] and heavy metal ions [8, 12].
The use of immobilized microorganisms rather than free cells in biodegradation can be advantageous to enhance the stability of the biocatalyst and to facilitate its recovery and reuse. Entrapment method as a traditional method is widely used in the immobilization of microorganisms . In our previous study, Sphingomonas sp. XLDN2-5 as a carbazole-degrading strain was entrapped in the mixture of Fe3O4 nanoparticles and gellan gum using modified traditional entrapment method . However, the mass-transfer problems of limited diffusion and steric hindrance reduced microbial cell access to substrate . Therefore, we constructed an efficient biocomposite by assembling Fe3O4 nanoparticles onto the surface of Sphingomonas sp. XLDN2-5 cells in this study. The resulting microbial cell/Fe3O4 biocomposite exhibited good biodegradation activity and reusability.
Analytical grade carbazole was purchased from Sigma-Aldrich (St. Louis, MO, USA). All other chemicals were of analytical grade and commercially available.
Sphingomonas sp. XLDN2-5, which can use carbazole as the sole source of carbon, nitrogen, and energy, was cultivated in the mineral salts medium (MSM) as previously described . Cells were harvested in the exponential phase (the optical density was about 0.68 to 0.70 at 620 nm) by centrifugation at 12,000 rpm for 10 min. The pellet was washed thrice with sodium chloride solution (0.9%, w/v) and then resuspended in sodium chloride solution (0.9%, w/v).
Fe3O4 nanoparticles were prepared as previously described . Fe3O4 powder (1.0 g) was put into 100 ml distilled water to form the Fe3O4 particle suspension. After ultrasonic disruption (25 KHz, 10 min; BUG25-06, Branson, MO, USA) of the suspension, the Fe3O4 nanoparticles were well dispersed in distilled water to form a stable suspension.
Fe3O4 particle suspension (1%, w/v) and cell suspension were mixed with the ratio of cell wet weight to Fe3O4 of 1 (w/w). Microbial cells and Fe3O4 nanoparticles were fully mixed by vortexing, then the mixture was incubated at 30°C for 2 h in a dark shaker to obtain microbial cell/Fe3O4 biocomposites.
All biodegradation experiments were carried out in 100-ml flasks containing 10-ml MSM at 30°C on a reciprocal shaker at 180 rpm. In each experiment, 3,500 μg of carbazole was added to MSM, and the microbial cell/Fe3O4 biocomposites made by 2 ml mixture of Fe3O4 particle suspension and cell suspension served as biocatalysts. Additionally, the same amount of cells was conducted in the batch biodegradation experiment. All the subsequent experiments contained the same amount of carbazole and biocatalysts as above.
In the recycle experiments, after each batch of biodegradation, the microbial cell/Fe3O4 biocomposites were collected using a magnetic field, and then were washed thrice with MSM to remove the free cells. After the MSM was drained, 10 ml of fresh MSM containing carbazole was added to repeat the cycle. All experiments were performed in triplicate.
After each batch of biodegradation, the biodegradation mixture was added 20 ml ethanol, followed by centrifugation (12,000 rpm for 20 min) and filtration. Residual contents of carbazole were determined using High-performance liquid chromatography (HPLC). HPLC was performed with an Agilent 1100 series (Hewlett-Packard) instrument equipped with a reversed-phase C18 column (4.6 mm × 150 mm, Hewlett-Packard). The mobile phase was a mixture of methanol and deionized water (90:10, v/v) at a flow rate of 0.5 ml min-1, and carbazole was monitored at 254 nm with a variable-wavelength detector.
The size and morphology of magnetic nanoparticles and microbial cell/Fe3O4 biocomposite were determined by transmission electronic microscopy (TEM; JEM-100cx II, JEOL, Akishima-shi, Japan). The sample was prepared by evaporating a drop of properly diluted microbial cell/Fe3O4 biocomposite or nanoparticle suspension on a carbon copper grid. The morphology of free cells was determined using a scanning electron microscope (SEM; S-570, Hitachi, Chiyoda-ku, Japan). Magnetization curves for the magnetic immobilized cells were obtained with a vibrating sample magnetometer (MicroMag 2900/3900, Princeton Measurements Corp., Westerville, OH, USA).
Results and discussion
Characteristics of microbial cell/Fe3O4 biocomposites
Biodegradation activity and reusability of microbial cell/Fe3O4 biocomposites
In an industrial bioremediation process, the recycle of the biocatalysts could be an important factor that determines the effectiveness of degradation for a long time. The carbazole biodegradation activities of microbial cell/Fe3O4 biocomposite were tested repeatedly. Each test was performed until the carbazole was consumed completely. At the end of each test, the microbial cell/Fe3O4 biocomposites were collected by application of a magnetic field and then reused in another test. As shown in Figure 4B, from the first to the sixth cycle, 3,500 μg carbazole was completely consumed by microbial cell/Fe3O4 biocomposite in 9 h; from the seventh to the tenth cycle, the same amount of carbazole was completely consumed in only 2 h. It was clear that the biodegradation activity of microbial cell/Fe3O4 biocomposites increased gradually during the recycling processes, which may be due to that more microbial cells was immobilized by Fe3O4 nanoparticles with the microbial cell growth and reproduction. Additionally, carbazole can be quickly transferred to the biocatalyst surface where nanosorbents were located and resulted in the increase of biodegradation rate [10, 14]. These results are different from other researchers' report which stated that the desulfurization activity of microbial cells coated by magnetite nanoparticles decreased gradually after a few test cycles .
In conclusion, the microbial cell/Fe3O4 biocomposite was evaluated as a novel aspect of the industrialization of microbial cell immobilization. Moreover, magnetic (Fe3O4) nanoparticles have a large specific surface and super-paramagnetic properties, which not only reduced the mass transfer resistance of traditional immobilization method, but also facilitated the recovery of immobilized cells in the reuse process. Additionally, the recycle experiments demonstrated that the biodegradation activity of microbial cell/Fe3O4 biocomposites increased gradually during the recycling processes. These results indicated that magnetically modified microbial cells provide a promising technique for improving biocatalysts used in the biodegradation of hazardous organic compounds.
This work was supported by grants from the National Natural Science Foundation of China (21177074), Excellent Middle-Aged and Youth Scientist Award Foundation of Shandong Province (BS2010SW016), and New Teacher Foundation of Ministry of Education of China (20090131120005).
- Benedik MJ, Gibbs PR, Riddle RR, Willson RC: Microbial denitrogenation of fossil fuels. Trends Biotechnol 1998, 16: 390–395. 10.1016/S0167-7799(98)01237-2View Article
- Jha AM, Bharti MK: Mutagenic profiles carbazole in the male germ cells of Swiss albino mice. Mutat Res 2002, 500: 97–101. 10.1016/S0027-5107(01)00303-7View Article
- O'Brien T, Schneider J, Warshawsky D, Mitchell K: In vitro toxicity of 7H-dibenzo[c, g]carbazole in human liver cell lines. Toxicol In Vitro 2002, 16: 235–243. 10.1016/S0887-2333(02)00013-9View Article
- Xu P, Yu B, Li FL, Cai XF, Ma CQ: Microbial degradation of sulfur, nitrogen and oxygen heterocycles. Trends Microbiol 2006, 14: 397–404.View Article
- Zhang WX: Nanoscale iron particles for environmental remediation: an overview. J Nanopart Res 2003, 5: 323–332. 10.1023/A:1025520116015View Article
- Kamat PV, Meisel D: Nanoscience opportunities in environmental remediation. Comptes Rendus Chimie 2003, 6: 999–1007. 10.1016/j.crci.2003.06.005View Article
- Wang X, Gai Z, Yu B, Feng J, Xu C, Yuan Y, Deng Z, Xu P: Degradation of carbazole by microbial cells immobilized in magnetic gellan gum gel beads. Appl Environ Microbiol 2007, 73: 6421–6428. 10.1128/AEM.01051-07View Article
- Wang X, Zhao C, Zhao P, Dou P, Ding Y, Xu P: Gellan gel beads containing magnetic nanoparticles: an effective biosorbent for the removal of heavy metals from aqueous system. Bioresour Technol 2009, 100: 2301–2304. 10.1016/j.biortech.2008.10.042View Article
- Tungittiplakorn W, Lion LW, Cohen C, Kim JY: Engineered polymeric nanoparticles for soil remediation. Environ Sci Technol 2004, 38: 1605–1610. 10.1021/es0348997View Article
- Shan GB, Zhang HY, Cai WQ, Xing JM, Liu HZ: Improvement of biodesulfurization rate by assembling nanosorbents on the surface of microbial cells. Biophys J 2005, 89: L58-L60. 10.1529/biophysj.105.073718View Article
- Shan GB, Xing JM, Zhang HY, Liu HZ: Biodesulfurization of dibenzothiophene by microbial cells coated with magnetic nanoparticles. Appl Environ Microbiol 2005, 71: 4497–4502. 10.1128/AEM.71.8.4497-4502.2005View Article
- Ponder SM, Darab JG, Mallouk TE: Remediation of Cr(VI) and Pb(II) aqueous solutions using supported nanoscale zero-valent iron. Environ Sci Technol 2000, 34: 2564–2569. 10.1021/es9911420View Article
- Park JK, Chang HN: Microencapsulation of microbial cells. Biotechnol Adv 2000, 18: 303–319. 10.1016/S0734-9750(00)00040-9View Article
- Safarik I, Safarikova M: Magnetically modified microbial cells: a new type of magnetic adsorbents. China Particuology 2007, 5: 519–525.View Article
- Gai ZH, Yu B, Li L, Wang Y, Ma CQ, Feng JH, Deng ZX, Xu P: Cometabolic degradation of dibenzofuran and dibenzothiophene by a newly isolated carbazole-degrading Sphingomonas sp. strain. Appl Environ Microbiol 2007, 73: 2832–2838. 10.1128/AEM.02704-06View Article
- Gupta AK, Gupta M: Synthesis and surface engineering of iron oxide nanoparticles for biomedical applications. Biomaterials 2005, 26: 3995–4021. 10.1016/j.biomaterials.2004.10.012View Article
- Lu AH, Salabas EL, Schüth F: Magnetic nanoparticles: sythesis, protection, functionalization, and application. Angew Chem Int Ed 2007, 46: 1222–1244. 10.1002/anie.200602866View Article
- Li YG, Gao HS, Li WL, Xing JM, Liu HZ: In situ magnetic separation and immobilization of dibenzothiophene-desulfurizing bacteria. Bioresour Technol 2009, 100: 5092–5096. 10.1016/j.biortech.2009.05.064View Article
- Safarikova M, Atanasova N, Ivanova V, Engibarov S, Weyda F, Tonkova A: Cyclodextrin glucanotransferase synthesis by semicontinuous cultivation of magnetic biocatalysts from cells of Bacillus circulans ATCC 21783. Process Biochem 2007, 42: 1454–1459. 10.1016/j.procbio.2007.06.009View Article
This article is published under license to BioMed Central Ltd. This is an open access article distributed under the terms of the Creative Commons Attribution License (http://creativecommons.org/licenses/by/2.0), which permits unrestricted use, distribution, and reproduction in any medium, provided the original work is properly cited.